Loading in 2 Seconds...
Loading in 2 Seconds...
LIVE‐CERAM experiment: Objectives and status of preparation. A. Miassoedov, X. Gaus-Liu , J. Foit, T. Cron, T. Wenz, S. Schmidt-Stiefel Karlsruhe Institute of Technology, Germany. Outline. Objectives of LIVE-CERAM experiment Difficulties in creating a 8 cm crust layer
Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.
A. Miassoedov, X. Gaus-Liu, J. Foit, T. Cron, T. Wenz, S. Schmidt-Stiefel
Karlsruhe Institute of Technology, Germany
Design of refractory liners for core catchers and for protection of concrete walls (applications for LWRs and for LMFBRs).
Development of model calculations for corium – refractory material interaction
Few data on corium-refractory material interaction
No detailed transient data available for the corium-refractory material interaction for 2D geometry
The objective is to simulate ablation process of a high-melting temperature refractory material by low-melting temperature corium
KNO3 as refractory material (melting temperature ~334°C) and a KNO3+NaNO3 melt at, initially, the eutectic composition (melting temperature ~220°C) as corium
Provide data for transientcorium-refractory material interaction
Evolution of boundary temperature during ablation transient
Evolution of melt pool temperature during ablation transient
A 8 cm KNO3 crust layer should be generated at the vessel wall.
8 heating elements
crust: 8 cm
crust profile in a volumetrically heated pool: thin and non-uniformly
desired crust profile in the LIVE-CERAM: thick and uniformly
multi-step melt extraction or
one-step melt extraction and heterogeneous heating
Geometries: height of refractory line: 435mm, height of ablation pool 385mm
Evolution of melt pool temperature: 36 thermocouples
Evolution of the interface temperature
Four thermocouple trees for crust temperature and interface temperature (new),
two positions for crust detection lance (new)
Initial ablation conditions: pouring temperature 260°C, maximum melt temperature 330°C, heating power 7kW in the liquid pool, vessel wall externally cooled by water
Steady-state criteria: steady melt temperature and crust temperature at polar angle 52° and 66°
Total heating power: 3300W at lower pool
Crust thickness: 6.5cm at top, maximum 14cm
Total heating power: 6200W, heterogeneous heating
Crust thickness: 6cm at top, 10cm at middle part and 11cm at bottom
The method of pre-test 3 (VV3) gives the best result.
A gap is formed between crust and wall due to crust shrinkage
The gap has a width about 1cm.
Most of the wall inner temperature thermocouples were destroyed during crust shrinkage.
The heat flux determination based on wall inner temperature will be not exact.
During ablation test, hot melt might penetrate through the crust to the gap and fill in the gap, so that the local heat transfer condition afterwards will be changed.
By filling the gap before the ablation test can decrease the width of the gap, but not completely get rid of it.
The plug temperatures at the wall can be used instead of the wall inner temperatures for the heat flux determination.
Instrumentation of 4 crust-temperature thermocouple trees, totally 63 pieces,
looking for the possibility of the second position for the melt/crust boundary temperature measurement with crust detection lance,
Waiting for the reply from CEA about
Confirmation of the method to create the refractory layer;
Confirmation of the instrumentations;
Opinion about the gap filling before the ablation test;
Confirmation of the participation of the test and the date of the test performance. The suitable date for KIT is November 28- December 09, 2011.